#------------------------------------------------------------------------------
#$Date: 2016-03-25 16:06:50 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179952 $
#$URL: svn://www.crystallography.net/cod/cif/7/02/47/7024713.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7024713
loop_
_publ_author_name
'Bobev, Svilen'
'Hullmann, Jonathan'
'Harmening, Thomas'
'Pöttgen, Rainer'
_publ_section_title
;
 Novel ternary alkaline-earth and rare-earth metal antimonides from
 gallium or indium flux. Synthesis, structural characterization and 121Sb
 and 151Eu Mössbauer spectroscopy of the series A7Ga8Sb8 (A = Sr, Ba,
 Eu) and Ba7In8Sb8.
;
_journal_issue                   26
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              6049
_journal_page_last               6055
_journal_paper_doi               10.1039/b920583g
_journal_volume                  39
_journal_year                    2010
_chemical_formula_moiety         'Eu0.88 Ga Sb'
_chemical_formula_sum            'Eu0.88 Ga Sb'
_chemical_formula_weight         324.43
_chemical_name_systematic
;
?
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            4
_cell_length_a                   4.4942(8)
_cell_length_b                   4.4942(8)
_cell_length_c                   17.274(6)
_cell_measurement_reflns_used    3024
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      26.9
_cell_measurement_theta_min      2.3
_cell_volume                     302.15(13)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      120(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0374
_diffrn_reflns_av_sigmaI/netI    0.0148
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            3024
_diffrn_reflns_theta_full        26.91
_diffrn_reflns_theta_max         26.91
_diffrn_reflns_theta_min         2.36
_exptl_absorpt_coefficient_mu    35.339
_exptl_absorpt_correction_T_max  0.2609
_exptl_absorpt_correction_T_min  0.1911
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS (Sheldrick, 2003)
;
_exptl_crystal_colour            grey
_exptl_crystal_density_diffrn    7.132
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       irregular
_exptl_crystal_F_000             549
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.851
_refine_diff_density_min         -2.144
_refine_diff_density_rms         0.316
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.282
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         160
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.282
_refine_ls_R_factor_all          0.0357
_refine_ls_R_factor_gt           0.0353
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+20.4087P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0769
_refine_ls_wR_factor_ref         0.0770
_reflns_number_gt                158
_reflns_number_total             160
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b920583g.txt
_cod_data_source_block           Eu0.875GaSb
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        302.16(13)
_cod_database_code               7024713
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z+1/2'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z-1/2'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Eu1 Eu 0.0000 0.0000 0.2500 0.0153(7) Uani 0.75 12 d SP
Eu2 Eu 0.0000 0.0000 0.0000 0.0172(6) Uani 1 12 d S
Sb1 Sb 0.3333 0.6667 0.12062(9) 0.0170(6) Uani 1 6 d S
Ga1 Ga 0.6667 0.3333 0.1562(4) 0.041(2) Uani 0.50 6 d SP
Ga2 Ga 0.8148(19) 0.1852(19) 0.2938(6) 0.036(3) Uani 0.17 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ga2 Eu1 Ga2 55.4(8) 16_456 1_455
Ga2 Eu1 Ga2 100.1(5) 16_456 17_546
Ga2 Eu1 Ga2 127.5(2) 1_455 17_546
Ga2 Eu1 Ga2 127.5(2) 16_456 3_665
Ga2 Eu1 Ga2 100.1(5) 1_455 3_665
Ga2 Eu1 Ga2 127.5(2) 17_546 3_665
Ga2 Eu1 Ga2 100.1(5) 16_456 18_666
Ga2 Eu1 Ga2 127.5(2) 1_455 18_666
Ga2 Eu1 Ga2 100.1(5) 17_546 18_666
Ga2 Eu1 Ga2 55.4(8) 3_665 18_666
Ga2 Eu1 Ga2 127.5(2) 16_456 2_545
Ga2 Eu1 Ga2 100.1(5) 1_455 2_545
Ga2 Eu1 Ga2 55.4(8) 17_546 2_545
Ga2 Eu1 Ga2 100.1(5) 3_665 2_545
Ga2 Eu1 Ga2 127.5(2) 18_666 2_545
Ga2 Eu1 Ga1 128.45(14) 16_456 16_556
Ga2 Eu1 Ga1 97.4(3) 1_455 16_556
Ga2 Eu1 Ga1 128.45(14) 17_546 16_556
Ga2 Eu1 Ga1 4.3(4) 3_665 16_556
Ga2 Eu1 Ga1 59.7(4) 18_666 16_556
Ga2 Eu1 Ga1 97.4(3) 2_545 16_556
Ga2 Eu1 Ga1 97.4(3) 16_456 1_445
Ga2 Eu1 Ga1 128.45(14) 1_455 1_445
Ga2 Eu1 Ga1 4.3(4) 17_546 1_445
Ga2 Eu1 Ga1 128.45(14) 3_665 1_445
Ga2 Eu1 Ga1 97.4(3) 18_666 1_445
Ga2 Eu1 Ga1 59.7(4) 2_545 1_445
Ga1 Eu1 Ga1 129.82(7) 16_556 1_445
Ga2 Eu1 Ga1 128.45(14) 16_456 16_446
Ga2 Eu1 Ga1 97.4(3) 1_455 16_446
Ga2 Eu1 Ga1 59.7(4) 17_546 16_446
Ga2 Eu1 Ga1 97.4(3) 3_665 16_446
Ga2 Eu1 Ga1 128.45(14) 18_666 16_446
Ga2 Eu1 Ga1 4.3(4) 2_545 16_446
Ga1 Eu1 Ga1 94.53(16) 16_556 16_446
Ga1 Eu1 Ga1 64.0(2) 1_445 16_446
Ga2 Eu1 Ga1 97.4(3) 16_456 .
Ga2 Eu1 Ga1 128.45(14) 1_455 .
Ga2 Eu1 Ga1 97.4(3) 17_546 .
Ga2 Eu1 Ga1 59.7(4) 3_665 .
Ga2 Eu1 Ga1 4.3(4) 18_666 .
Ga2 Eu1 Ga1 128.45(14) 2_545 .
Ga1 Eu1 Ga1 64.0(2) 16_556 .
Ga1 Eu1 Ga1 94.53(16) 1_445 .
Ga1 Eu1 Ga1 129.82(7) 16_446 .
Ga2 Eu1 Ga1 59.7(4) 16_456 16_456
Ga2 Eu1 Ga1 4.3(4) 1_455 16_456
Ga2 Eu1 Ga1 128.45(14) 17_546 16_456
Ga2 Eu1 Ga1 97.4(3) 3_665 16_456
Ga2 Eu1 Ga1 128.45(14) 18_666 16_456
Ga2 Eu1 Ga1 97.4(3) 2_545 16_456
Ga1 Eu1 Ga1 94.53(16) 16_556 16_456
Ga1 Eu1 Ga1 129.82(7) 1_445 16_456
Ga1 Eu1 Ga1 94.53(16) 16_446 16_456
Ga1 Eu1 Ga1 129.82(7) . 16_456
Ga2 Eu1 Ga1 4.3(4) 16_456 1_455
Ga2 Eu1 Ga1 59.7(4) 1_455 1_455
Ga2 Eu1 Ga1 97.4(3) 17_546 1_455
Ga2 Eu1 Ga1 128.45(14) 3_665 1_455
Ga2 Eu1 Ga1 97.4(3) 18_666 1_455
Ga2 Eu1 Ga1 128.45(14) 2_545 1_455
Ga1 Eu1 Ga1 129.82(7) 16_556 1_455
Ga1 Eu1 Ga1 94.53(16) 1_445 1_455
Ga1 Eu1 Ga1 129.82(7) 16_446 1_455
Ga1 Eu1 Ga1 94.53(16) . 1_455
Ga1 Eu1 Ga1 64.0(2) 16_456 1_455
Sb1 Eu2 Sb1 84.95(3) 13 13_665
Sb1 Eu2 Sb1 95.05(3) 13 1_445
Sb1 Eu2 Sb1 180.00(4) 13_665 1_445
Sb1 Eu2 Sb1 84.95(3) 13 13_565
Sb1 Eu2 Sb1 84.95(3) 13_665 13_565
Sb1 Eu2 Sb1 95.05(3) 1_445 13_565
Sb1 Eu2 Sb1 95.05(3) 13 1_545
Sb1 Eu2 Sb1 95.05(3) 13_665 1_545
Sb1 Eu2 Sb1 84.95(3) 1_445 1_545
Sb1 Eu2 Sb1 180.00(4) 13_565 1_545
Sb1 Eu2 Sb1 180.0 13 .
Sb1 Eu2 Sb1 95.05(3) 13_665 .
Sb1 Eu2 Sb1 84.95(3) 1_445 .
Sb1 Eu2 Sb1 95.05(3) 13_565 .
Sb1 Eu2 Sb1 84.95(3) 1_545 .
Sb1 Eu2 Ga1 136.18(2) 13 .
Sb1 Eu2 Ga1 84.88(9) 13_665 .
Sb1 Eu2 Ga1 95.12(9) 1_445 .
Sb1 Eu2 Ga1 136.18(2) 13_565 .
Sb1 Eu2 Ga1 43.82(2) 1_545 .
Sb1 Eu2 Ga1 43.82(2) . .
Sb1 Eu2 Ga1 43.82(2) 13 13
Sb1 Eu2 Ga1 95.12(9) 13_665 13
Sb1 Eu2 Ga1 84.88(9) 1_445 13
Sb1 Eu2 Ga1 43.82(2) 13_565 13
Sb1 Eu2 Ga1 136.18(2) 1_545 13
Sb1 Eu2 Ga1 136.18(2) . 13
Ga1 Eu2 Ga1 180.0 . 13
Sb1 Eu2 Ga1 95.12(9) 13 13_665
Sb1 Eu2 Ga1 43.82(2) 13_665 13_665
Sb1 Eu2 Ga1 136.18(2) 1_445 13_665
Sb1 Eu2 Ga1 43.82(2) 13_565 13_665
Sb1 Eu2 Ga1 136.18(2) 1_545 13_665
Sb1 Eu2 Ga1 84.88(9) . 13_665
Ga1 Eu2 Ga1 106.21(13) . 13_665
Ga1 Eu2 Ga1 73.79(13) 13 13_665
Sb1 Eu2 Ga1 84.88(9) 13 1_445
Sb1 Eu2 Ga1 136.18(2) 13_665 1_445
Sb1 Eu2 Ga1 43.82(2) 1_445 1_445
Sb1 Eu2 Ga1 136.18(2) 13_565 1_445
Sb1 Eu2 Ga1 43.82(2) 1_545 1_445
Sb1 Eu2 Ga1 95.12(9) . 1_445
Ga1 Eu2 Ga1 73.79(13) . 1_445
Ga1 Eu2 Ga1 106.21(13) 13 1_445
Ga1 Eu2 Ga1 180.00(16) 13_665 1_445
Sb1 Eu2 Ga1 43.82(2) 13 13_655
Sb1 Eu2 Ga1 43.82(2) 13_665 13_655
Sb1 Eu2 Ga1 136.18(2) 1_445 13_655
Sb1 Eu2 Ga1 95.12(9) 13_565 13_655
Sb1 Eu2 Ga1 84.88(9) 1_545 13_655
Sb1 Eu2 Ga1 136.18(2) . 13_655
Ga1 Eu2 Ga1 106.21(13) . 13_655
Ga1 Eu2 Ga1 73.79(13) 13 13_655
Ga1 Eu2 Ga1 73.79(13) 13_665 13_655
Ga1 Eu2 Ga1 106.21(13) 1_445 13_655
Sb1 Eu2 Ga1 136.18(2) 13 1_455
Sb1 Eu2 Ga1 136.18(2) 13_665 1_455
Sb1 Eu2 Ga1 43.82(2) 1_445 1_455
Sb1 Eu2 Ga1 84.88(9) 13_565 1_455
Sb1 Eu2 Ga1 95.12(9) 1_545 1_455
Sb1 Eu2 Ga1 43.82(2) . 1_455
Ga1 Eu2 Ga1 73.79(13) . 1_455
Ga1 Eu2 Ga1 106.21(13) 13 1_455
Ga1 Eu2 Ga1 106.21(13) 13_665 1_455
Ga1 Eu2 Ga1 73.79(13) 1_445 1_455
Ga1 Eu2 Ga1 180.00(16) 13_655 1_455
Ga1 Sb1 Ga1 114.86(12) . 1_565
Ga1 Sb1 Ga1 114.86(12) . 1_455
Ga1 Sb1 Ga1 114.86(12) 1_565 1_455
Ga1 Sb1 Ga2 123.4(3) . 18_676
Ga1 Sb1 Ga2 31.2(3) 1_565 18_676
Ga1 Sb1 Ga2 85.7(3) 1_455 18_676
Ga1 Sb1 Ga2 123.4(3) . 17_556
Ga1 Sb1 Ga2 85.7(3) 1_565 17_556
Ga1 Sb1 Ga2 31.2(3) 1_455 17_556
Ga2 Sb1 Ga2 55.2(6) 18_676 17_556
Ga1 Sb1 Ga2 85.7(3) . 16_566
Ga1 Sb1 Ga2 31.2(3) 1_565 16_566
Ga1 Sb1 Ga2 123.4(3) 1_455 16_566
Ga2 Sb1 Ga2 43.5(6) 18_676 16_566
Ga2 Sb1 Ga2 92.8(3) 17_556 16_566
Ga1 Sb1 Ga2 85.7(3) . 16_456
Ga1 Sb1 Ga2 123.4(3) 1_565 16_456
Ga1 Sb1 Ga2 31.2(3) 1_455 16_456
Ga2 Sb1 Ga2 92.8(3) 18_676 16_456
Ga2 Sb1 Ga2 43.5(6) 17_556 16_456
Ga2 Sb1 Ga2 113.1(4) 16_566 16_456
Ga1 Sb1 Ga2 31.2(3) . 17_656
Ga1 Sb1 Ga2 85.7(3) 1_565 17_656
Ga1 Sb1 Ga2 123.4(3) 1_455 17_656
Ga2 Sb1 Ga2 92.8(3) 18_676 17_656
Ga2 Sb1 Ga2 113.1(4) 17_556 17_656
Ga2 Sb1 Ga2 55.2(6) 16_566 17_656
Ga2 Sb1 Ga2 92.8(3) 16_456 17_656
Ga1 Sb1 Ga2 31.2(3) . 18_666
Ga1 Sb1 Ga2 123.4(3) 1_565 18_666
Ga1 Sb1 Ga2 85.7(3) 1_455 18_666
Ga2 Sb1 Ga2 113.1(4) 18_676 18_666
Ga2 Sb1 Ga2 92.8(3) 17_556 18_666
Ga2 Sb1 Ga2 92.8(3) 16_566 18_666
Ga2 Sb1 Ga2 55.2(6) 16_456 18_666
Ga2 Sb1 Ga2 43.5(6) 17_656 18_666
Ga1 Sb1 Eu2 76.40(11) . .
Ga1 Sb1 Eu2 154.55(16) 1_565 .
Ga1 Sb1 Eu2 76.40(11) 1_455 .
Ga2 Sb1 Eu2 158.1(3) 18_676 .
Ga2 Sb1 Eu2 107.6(3) 17_556 .
Ga2 Sb1 Eu2 158.1(3) 16_566 .
Ga2 Sb1 Eu2 78.5(2) 16_456 .
Ga2 Sb1 Eu2 107.6(3) 17_656 .
Ga2 Sb1 Eu2 78.5(2) 18_666 .
Ga1 Sb1 Eu2 154.55(16) . 1_565
Ga1 Sb1 Eu2 76.40(11) 1_565 1_565
Ga1 Sb1 Eu2 76.40(11) 1_455 1_565
Ga2 Sb1 Eu2 78.5(2) 18_676 1_565
Ga2 Sb1 Eu2 78.5(2) 17_556 1_565
Ga2 Sb1 Eu2 107.6(3) 16_566 1_565
Ga2 Sb1 Eu2 107.6(3) 16_456 1_565
Ga2 Sb1 Eu2 158.1(3) 17_656 1_565
Ga2 Sb1 Eu2 158.1(3) 18_666 1_565
Eu2 Sb1 Eu2 84.95(3) . 1_565
Ga1 Sb1 Eu2 76.40(11) . 1_665
Ga1 Sb1 Eu2 76.40(11) 1_565 1_665
Ga1 Sb1 Eu2 154.55(16) 1_455 1_665
Ga2 Sb1 Eu2 107.6(3) 18_676 1_665
Ga2 Sb1 Eu2 158.1(3) 17_556 1_665
Ga2 Sb1 Eu2 78.5(2) 16_566 1_665
Ga2 Sb1 Eu2 158.1(3) 16_456 1_665
Ga2 Sb1 Eu2 78.5(2) 17_656 1_665
Ga2 Sb1 Eu2 107.6(3) 18_666 1_665
Eu2 Sb1 Eu2 84.95(3) . 1_665
Eu2 Sb1 Eu2 84.95(3) 1_565 1_665
Ga2 Ga1 Ga2 87.8(8) 17_656 18_666
Ga2 Ga1 Ga2 87.8(8) 17_656 16_556
Ga2 Ga1 Ga2 87.8(8) 18_666 16_556
Ga2 Ga1 Ga2 27.3(5) 17_656 2_655
Ga2 Ga1 Ga2 68.6(6) 18_666 2_655
Ga2 Ga1 Ga2 68.6(6) 16_556 2_655
Ga2 Ga1 Ga2 68.6(6) 17_656 3_665
Ga2 Ga1 Ga2 27.3(5) 18_666 3_665
Ga2 Ga1 Ga2 68.6(6) 16_556 3_665
Ga2 Ga1 Ga2 44.4(5) 2_655 3_665
Ga2 Ga1 Ga2 68.6(6) 17_656 .
Ga2 Ga1 Ga2 68.6(6) 18_666 .
Ga2 Ga1 Ga2 27.3(5) 16_556 .
Ga2 Ga1 Ga2 44.4(5) 2_655 .
Ga2 Ga1 Ga2 44.4(5) 3_665 .
Ga2 Ga1 Sb1 75.4(2) 17_656 .
Ga2 Ga1 Sb1 75.4(2) 18_666 .
Ga2 Ga1 Sb1 156.5(6) 16_556 .
Ga2 Ga1 Sb1 89.7(2) 2_655 .
Ga2 Ga1 Sb1 89.7(2) 3_665 .
Ga2 Ga1 Sb1 129.2(4) . .
Ga2 Ga1 Sb1 156.5(6) 17_656 1_545
Ga2 Ga1 Sb1 75.4(2) 18_666 1_545
Ga2 Ga1 Sb1 75.4(2) 16_556 1_545
Ga2 Ga1 Sb1 129.2(4) 2_655 1_545
Ga2 Ga1 Sb1 89.7(2) 3_665 1_545
Ga2 Ga1 Sb1 89.7(2) . 1_545
Sb1 Ga1 Sb1 114.86(12) . 1_545
Ga2 Ga1 Sb1 75.4(2) 17_656 1_655
Ga2 Ga1 Sb1 156.5(6) 18_666 1_655
Ga2 Ga1 Sb1 75.4(2) 16_556 1_655
Ga2 Ga1 Sb1 89.7(2) 2_655 1_655
Ga2 Ga1 Sb1 129.2(4) 3_665 1_655
Ga2 Ga1 Sb1 89.7(2) . 1_655
Sb1 Ga1 Sb1 114.86(12) . 1_655
Sb1 Ga1 Sb1 114.86(12) 1_545 1_655
Ga2 Ga1 Eu1 4.8(5) 17_656 1_665
Ga2 Ga1 Eu1 91.2(4) 18_666 1_665
Ga2 Ga1 Eu1 91.2(4) 16_556 1_665
Ga2 Ga1 Eu1 32.1(3) 2_655 1_665
Ga2 Ga1 Eu1 73.0(3) 3_665 1_665
Ga2 Ga1 Eu1 73.0(3) . 1_665
Sb1 Ga1 Eu1 73.10(5) . 1_665
Sb1 Ga1 Eu1 161.3(3) 1_545 1_665
Sb1 Ga1 Eu1 73.10(5) 1_655 1_665
Ga2 Ga1 Eu1 91.2(4) 17_656 1_655
Ga2 Ga1 Eu1 91.2(4) 18_666 1_655
Ga2 Ga1 Eu1 4.8(5) 16_556 1_655
Ga2 Ga1 Eu1 73.0(3) 2_655 1_655
Ga2 Ga1 Eu1 73.0(3) 3_665 1_655
Ga2 Ga1 Eu1 32.1(3) . 1_655
Sb1 Ga1 Eu1 161.3(3) . 1_655
Sb1 Ga1 Eu1 73.10(5) 1_545 1_655
Sb1 Ga1 Eu1 73.10(5) 1_655 1_655
Eu1 Ga1 Eu1 94.53(16) 1_665 1_655
Ga2 Ga1 Eu1 91.2(4) 17_656 .
Ga2 Ga1 Eu1 4.8(5) 18_666 .
Ga2 Ga1 Eu1 91.2(4) 16_556 .
Ga2 Ga1 Eu1 73.0(3) 2_655 .
Ga2 Ga1 Eu1 32.1(3) 3_665 .
Ga2 Ga1 Eu1 73.0(3) . .
Sb1 Ga1 Eu1 73.10(5) . .
Sb1 Ga1 Eu1 73.10(5) 1_545 .
Sb1 Ga1 Eu1 161.3(3) 1_655 .
Eu1 Ga1 Eu1 94.53(16) 1_665 .
Eu1 Ga1 Eu1 94.53(16) 1_655 .
Ga1 Ga2 Ga2 126.8(5) 16_556 16_556
Ga1 Ga2 Eu1 170.9(9) 16_556 1_655
Ga2 Ga2 Eu1 62.3(4) 16_556 1_655
Ga1 Ga2 Ga2 46.1(4) 16_556 3_665
Ga2 Ga2 Ga2 89.999(2) 16_556 3_665
Eu1 Ga2 Ga2 140.1(3) 1_655 3_665
Ga1 Ga2 Ga2 46.1(4) 16_556 2_655
Ga2 Ga2 Ga2 89.999(2) 16_556 2_655
Eu1 Ga2 Ga2 140.1(3) 1_655 2_655
Ga2 Ga2 Ga2 60.001(7) 3_665 2_655
Ga1 Ga2 Ga2 133.9(4) 16_556 3_765
Ga2 Ga2 Ga2 89.998(2) 16_556 3_765
Eu1 Ga2 Ga2 39.9(2) 1_655 3_765
Ga2 Ga2 Ga2 179.998(16) 3_665 3_765
Ga2 Ga2 Ga2 120.000(4) 2_655 3_765
Ga1 Ga2 Ga2 133.9(4) 16_556 2_645
Ga2 Ga2 Ga2 89.998(2) 16_556 2_645
Eu1 Ga2 Ga2 39.9(2) 1_655 2_645
Ga2 Ga2 Ga2 120.000(4) 3_665 2_645
Ga2 Ga2 Ga2 179.998(4) 2_655 2_645
Ga2 Ga2 Ga2 60.000(2) 3_765 2_645
Ga1 Ga2 Ga2 79.0(7) 16_556 18_666
Ga2 Ga2 Ga2 52.8(5) 16_556 18_666
Eu1 Ga2 Ga2 109.3(6) 1_655 18_666
Ga2 Ga2 Ga2 37.2(5) 3_665 18_666
Ga2 Ga2 Ga2 66.52(17) 2_655 18_666
Ga2 Ga2 Ga2 142.8(5) 3_765 18_666
Ga2 Ga2 Ga2 113.48(18) 2_645 18_666
Ga1 Ga2 Ga2 79.0(7) 16_556 17_656
Ga2 Ga2 Ga2 52.8(5) 16_556 17_656
Eu1 Ga2 Ga2 109.3(6) 1_655 17_656
Ga2 Ga2 Ga2 66.52(17) 3_665 17_656
Ga2 Ga2 Ga2 37.2(5) 2_655 17_656
Ga2 Ga2 Ga2 113.48(18) 3_765 17_656
Ga2 Ga2 Ga2 142.8(5) 2_645 17_656
Ga2 Ga2 Ga2 47.0(4) 18_666 17_656
Ga1 Ga2 Ga1 101.0(7) 16_556 .
Ga2 Ga2 Ga1 25.9(3) 16_556 .
Eu1 Ga2 Ga1 88.2(4) 1_655 .
Ga2 Ga2 Ga1 67.8(3) 3_665 .
Ga2 Ga2 Ga1 67.8(3) 2_655 .
Ga2 Ga2 Ga1 112.2(3) 3_765 .
Ga2 Ga2 Ga1 112.2(3) 2_645 .
Ga2 Ga2 Ga1 32.4(3) 18_666 .
Ga2 Ga2 Ga1 32.4(3) 17_656 .
Ga1 Ga2 Sb1 73.4(3) 16_556 16_656
Ga2 Ga2 Sb1 123.27(19) 16_556 16_656
Eu1 Ga2 Sb1 102.0(4) 1_655 16_656
Ga2 Ga2 Sb1 117.6(3) 3_665 16_656
Ga2 Ga2 Sb1 68.2(3) 2_655 16_656
Ga2 Ga2 Sb1 62.4(3) 3_765 16_656
Ga2 Ga2 Sb1 111.8(3) 2_645 16_656
Ga2 Ga2 Sb1 134.5(4) 18_666 16_656
Ga2 Ga2 Sb1 92.1(5) 17_656 16_656
Ga1 Ga2 Sb1 121.1(2) . 16_656
Ga1 Ga2 Sb1 73.4(3) 16_556 16_546
Ga2 Ga2 Sb1 123.27(19) 16_556 16_546
Eu1 Ga2 Sb1 102.0(4) 1_655 16_546
Ga2 Ga2 Sb1 68.2(3) 3_665 16_546
Ga2 Ga2 Sb1 117.6(3) 2_655 16_546
Ga2 Ga2 Sb1 111.8(3) 3_765 16_546
Ga2 Ga2 Sb1 62.4(3) 2_645 16_546
Ga2 Ga2 Sb1 92.1(5) 18_666 16_546
Ga2 Ga2 Sb1 134.5(4) 17_656 16_546
Ga1 Ga2 Sb1 121.1(2) . 16_546
Sb1 Ga2 Sb1 113.1(4) 16_656 16_546
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Eu1 Ga2 1.628(14) 16_456
Eu1 Ga2 1.628(14) 1_455
Eu1 Ga2 1.628(14) 17_546
Eu1 Ga2 1.628(14) 3_665
Eu1 Ga2 1.628(14) 18_666
Eu1 Ga2 1.628(14) 2_545
Eu1 Ga1 3.059(4) 16_556
Eu1 Ga1 3.059(4) 1_445
Eu1 Ga1 3.059(4) 16_446
Eu1 Ga1 3.059(4) .
Eu1 Ga1 3.059(4) 16_456
Eu1 Ga1 3.059(4) 1_455
Eu2 Sb1 3.3277(11) 13
Eu2 Sb1 3.3277(11) 13_665
Eu2 Sb1 3.3277(11) 1_445
Eu2 Sb1 3.3277(11) 13_565
Eu2 Sb1 3.3277(11) 1_545
Eu2 Sb1 3.3277(11) .
Eu2 Ga1 3.743(5) .
Eu2 Ga1 3.743(5) 13
Eu2 Ga1 3.743(5) 13_665
Eu2 Ga1 3.743(5) 1_445
Eu2 Ga1 3.743(5) 13_655
Eu2 Ga1 3.743(5) 1_455
Sb1 Ga1 2.6664(18) .
Sb1 Ga1 2.6664(18) 1_565
Sb1 Ga1 2.6664(18) 1_455
Sb1 Ga2 2.693(6) 18_676
Sb1 Ga2 2.693(6) 17_556
Sb1 Ga2 2.693(6) 16_566
Sb1 Ga2 2.693(6) 16_456
Sb1 Ga2 2.693(6) 17_656
Sb1 Ga2 2.693(6) 18_666
Sb1 Eu2 3.3277(11) 1_565
Sb1 Eu2 3.3277(11) 1_665
Ga1 Ga2 1.441(14) 17_656
Ga1 Ga2 1.441(14) 18_666
Ga1 Ga2 1.441(14) 16_556
Ga1 Ga2 2.643(13) 2_655
Ga1 Ga2 2.643(13) 3_665
Ga1 Ga2 2.643(13) .
Ga1 Sb1 2.6664(18) 1_545
Ga1 Sb1 2.6664(18) 1_655
Ga1 Eu1 3.059(4) 1_665
Ga1 Eu1 3.059(4) 1_655
Ga2 Ga1 1.441(14) 16_556
Ga2 Ga2 1.51(2) 16_556
Ga2 Eu1 1.629(14) 1_655
Ga2 Ga2 2.00(3) 3_665
Ga2 Ga2 2.00(3) 2_655
Ga2 Ga2 2.50(3) 3_765
Ga2 Ga2 2.50(3) 2_645
Ga2 Ga2 2.51(2) 18_666
Ga2 Ga2 2.51(2) 17_656
Ga2 Sb1 2.693(6) 16_656
Ga2 Sb1 2.693(6) 16_546
